Journal of CO2 Utilization 17 (2017) 273–283 Contents lists available at ScienceDirect Journal of CO2 Utilization journal homepage: www.elsevier.com/locate/jcou Co-synthesis of methanol and methyl formate from CO2 hydrogenation over oxalate ligand functionalized ZSM-5 supported Cu/ZnO catalyst Olumide Bolarinwa Ayodelea,b,* , Sara Faiz Hanna Tasfyc , Noor Asmawati Mohd Zabidid , Yoshimitsu Uemurab a Department of Chemical Engineering, Universiti Teknologi PETRONAS, 32610, Bandar, Seri Iskandar, Perak, Malaysia Centre for Biofuel and Biochemical Research, Universiti Teknologi PETRONAS, 32610, Bandar, Seri Iskandar, Perak, Malaysia Department of Chemical and Petroleum Engineering, American University of Ras Al Khaimah, 10021 Ras Al Khaimah, UAE d Department of Fundamental and Applied Sciences, Universiti Teknologi PETRONAS, 32610 Seri Iskandar, Perak, Malaysia b c A R T I C L E I N F O Article history: Received 20 September 2016 Received in revised form 8 November 2016 Accepted 19 November 2016 Available online xxx Keywords: CO2 hydrogenation Oxalate ligand functionalization Methanol Methyl formate ZSM-5 A B S T R A C T Co-synthesis of methanol and methyl formate (MF) was achieved in this study using expediently synthesized ZSM-5 supported oxalate ligand functionalized Cu/ZnO catalyst (CZOx/Z) in a continuous ﬂow reactor. The catalyst characterization results showed that the synthesis protocol via oxalate ligand functionalization (OLF) achieved considerable reduction of CuO ! Cu2O ! Cu leading to highly reducible active metals with largely weak metal-support-interactions according to the X-ray photoelectron spectroscopy, Raman spectroscopy and temperature programmed reduction. The ZnO reduction peak was also observed to shift to lower reduction temperature. Furthermore, the NH3- and CO2- temperature programmed desorption studies showed that CZOx/Z has both acid and basic sites, but the acid sites were about four times higher. These qualities were ascribed to the OLF at the synthesis stage which also guarantees ultraﬁne active metal particle sizes with high degree of dispersion. The CZOx/Z showed exceptional CO2 hydrogenation activity at 250 C and 2.25 MPa, the initial CO2 conversion increased marginally from 15.5 to 15.9% in the ﬁrst 180 min and increased to 20.5% at 600 min time-on-stream. The increment was ascribed to reduction of remnant unreduced active metal species with methanol which simultaneously proceeds with dehydrogenation of produced methanol to form MF promoted by the acid sites. The methanol selectivity was 97.16% at 60 min TOS and later decreased to 64.64% at 180 min as the formation of MF increased owing to the progressive reduction of active metals with formed methanol. CZOx/Z is a promising catalyst for co-synthesis of methanol and MF. © 2016 Elsevier Ltd. All rights reserved. 1. Introduction As the world battles both energy challenge for the future and effect of greenhouse gases upon combustion of fossil fuel, attention is shifting drastically to several alternative fuels that are environmental friendly and economically suitable and sustainable. Key alternatives include biofuels produced via hydrodeoxygenation which we have in recent times been extensively reported [1– 5]. Another area that is currently receiving tremendous attention is methanol synthesis from CO2 hydrogenation . The process does not only mop up CO2 thus mitigating the greenhouse effects, but it is also a viable strategy to transport hydrogen gas energy produced * Corresponding author at: Department of Chemical Engineering, Universiti Teknologi PETRONAS, 32610, Bandar, Seri Iskandar, Perak, Malaysia. E-mail address: [email protected] (O.B. Ayodele). http://dx.doi.org/10.1016/j.jcou.2016.11.016 2212-9820/© 2016 Elsevier Ltd. All rights reserved. from natural means such as solar energy and hydropower. In addition, methanol has played a vital role as chemical feedstock for several important chemicals such as methyl tert-butyl ether (MTBE), acetic acid, formaldehyde, and chloromethane for over four decades as well as acting as a high-density hydrogen carrier for different types of fuel cells [7,8]. Typically, methanol is produced at the industrial scale from a mixture of synthesis gas (CO/CO2/H2) at elevated pressures (50–100 bar) and temperatures (200–300 C) over Cu/ZnO/Al2O3 catalysts with an estimated annual global production of 50 million tons . There is a unanimous consensus in the literature that Cu/ZnO (with Cu-rich molar compositions of Cu:Zn near 70:30) combination is excellent for production of methanol via hydrogenation of CO2 route [6,7,9–11], although there are few other reports that discuss the application of other metals such as Mo and Pd [12,13] and metal oxide such as In2O3 . In all these recent reports, catalyst synthesis and reactivity studies appear to be at the fore, in 274 O.B. Ayodele et al. / Journal of CO2 Utilization 17 (2017) 273–283 fact, Behrens et al.  and da Silva  noted that the phenomenological optimization of the preparation of catalytically very active “methanol copper” with support such as Nb2O5 and increased acidity is far more advanced than the fundamental understanding of its high catalytic activity. Therefore, the modiﬁcation and optimization of catalysts have been a key research to improve both CO2 conversion and methanol selectivity. The reaction mechanism of industrial methanol synthesis as well as the nature of the active site on Cu/ZnO based high-performance catalysts have been debated and are still not comprehensively understood . Different literature have argued that active sites over the Cu-based catalysts for CO2 hydrogenation to methanol were Cu0 or Cu+, some also reported that both Cu0 and Cu+ were effective for the CO2 hydrogenation to methanol [6,10]. For example, Natesakhawat et al. , reported that metallic Cu is the active site, and in fact the activity is found to be directly proportional to the Cu0 surface area. This opinion was also corroborated by the recent study of Witoon et al. . Generally in the literature, active metal/metal oxide dispersion, reducibility, and metal particle sizes have signiﬁcant inﬂuence on the formulated Cu/ZnO catalyst. Among the earliest methods to achieve these was the introduction of catalyst promoters such as Zr, Ga, Nb, Cr, Th etc. [7,14,16–22], however active metal sintering was a signiﬁcant limitation due to the effect of high temperature during H2 reduction process to activate the catalyst . In order to achieve high reducibility and prevent unwanted active metal agglomeration which can cause fast growth of particles during the conventional H2 or CO reduction process for metal oxides especially at high temperature, chemical treatment methods using NaBH4 has been considered . The method was considered effective especially considering the characteristics of intense heating effect, time-consuming operation and unmanageable reducing conditions, which could lead to sintering of active metals . Belin et al.  found that catalysts prepared by coimpregnation of HAuCl4 and Cu(NO3)2 and reduced with NaBH4 solution leads to smaller particles with negligible interaction between copper and gold leading to higher activity and selectivity, while the catalysts reduced with hydrogen at higher temperature showed a signiﬁcant level of CuAu alloy, thus exhibiting lower activity and selectivity. In another report by Liaw and Chen , modiﬁcation of the Cu catalyst with NaBH4 solution achieved 100% reduction of CuO to Cu0, in addition, the catalysts particles were ultraﬁne with superior activity and methanol selectivity compared to Cu catalyst reduced with H2. Another interesting study was reported by Fujita et al. which showed that methanol was a better reducing agent than H2 in CO2 hydrogenation to methanol . Their report showed that methanol reduction produces high dispersion of Cu with preferential emergence of ﬂat surface Cu sites which resulted into higher activity and higher methanol selectivity. In all these studies, CO is a major by-product and in most cases it is the only by-product which according to the report of Chen et al.  is produced via parallel formate dissociation mechanism. Thus, it is enticing to design catalysts that can produce a value added by-products such as methyl formate (MF). MF is the simplest carboxylate ester and it has wide range of applications in chemical industries like in the production of formic acid derivatives, blowing agent for foams, and as an agricultural fumigant. Its laboratory synthesis is usually via acid catalyzed esteriﬁcation of formic acid and methanol, while it is produced industrially by the base-catalyzed reaction of methanol and carbon monoxide . Recently we reported the effect of organic ligand functionalization on alumina supported nickel catalysts (NiOx/Al2O3) for the hydrodeoxygenation of oleic acid into biofuel . The characterization results showed that the number of Ni species active sites is higher in NiOx/Al2O3 than the conventional (Ni/Al2O3) catalyst. In addition, NiOx/Al2O3 exhibited higher Ni dispersion with weaker metal-support-interaction leading to highly reducible NiO with comparable smaller particle sizes. Furthermore, their catalytic activities showed that NiOx/Al2O3 has the highest rate constants but the least activation energy of 176 kJ/mol compared to 244 kJ/ mol evaluated when using Ni/Al2O3. In all the surveyed literature, functionalization of Cu/ZnO catalyst with organic ligands such as oxalate for CO2 hydrogenation to methanol is rarely found except for the study of Jingfa et al.  and Ning et al.  where the catalyst was prepared by oxalate gel-co-precipitation using ethanol as solvent. In both studies, the catalysts that were prepared via oxalate gel-co-precipitation showed reduced homogeneous Cu and Zn particle sizes distribution, increased CO2 conversion and higher methanol selectivity compared to catalysts synthesized via conventional carbonate salts as co-precipitation agents. Therefore in this study, we investigate the applicability of functionalizing Cu and Zn with oxalate ligand using oxalic acid for the CO2 hydrogenation to methanol. The catalyst was supported on ZSM-5, a rarely used support, and expediently characterized and tested for CO2 hydrogenation to methanol and the results were meticulously compared to leading research reports in the literature. The catalyst did not only show superior activity and selectivity compared to literature reports, it also produces high yield of MF without signiﬁcantly compromising the yield of methanol. 2. Experimental 2.1. Materials Both Cu(NO3)23H2O (Mwt: 241.6, 99.0%) and Zn(NO3)26H2O (Mwt 297.49, 99.0%) that were used as the catalyst precursor were purchased from Sigma Aldrich, while oxalic acid (OxA) and ZSM-5 were purchased from Spectrum chemicals. 2.2. Catalyst synthesis The synthesis of Cu/Zn (70:30) for the CO2 hydrogenation was achieved in two successive stages. In the ﬁrst stage, copper oxalate (CuOx) and zinc oxalate (ZnOx) catalyst precursors were synthesized by reacting 7.98 g Cu(NO3)23H2O and 4.1 g Zn(NO3)26H2O separately with aqueous oxalic acid (OxA) in stoichiometry ratios under vigorous stirring for 30 min at 60 C in different conical ﬂask. The ﬂasks were wrapped with aluminum foil since metal oxalates are photo-sentitive . The pH of CuOx and ZnOx were observed to be 2.5 and 4.2, respectively. In the second step, both CuOx and ZnOx were slowly added to 20 g ZSM-5 dispersion under continuous stirring at 70 C for 6 h to ensure their complete incorporation into the ZSM-5 support. The total amount of metals incorporated into the ZSM-5 supported oxalate ligand functionalized Cu and Zn (CZOx/Z) catalyst were calculated to be 15%. The CZOx/Z was dried in the oven at 105 C for 12 h, grinded and calcined at 350 C for 4 h with a slow temperature ramping of 4 C min1. 2.3. Catalyst characterization Extreme high resolution ﬁeld emission scanning electron microscope (XHR-FESEM) and energy dispersive X-ray (EDX) were performed to determine the samples morphology and elemental composition, respectively using Verios XHR-FESEM (Model 460L, FEITM) equipped with an EDS detector. The catalyst microstructure and crystallographic information were studied by high resolution transmission electron microscope (HRTEM) 200 kV with Field Emission (TECNAI G2 20 S-TWIN, FEITM). X-ray diffraction (XRD) O.B. Ayodele et al. / Journal of CO2 Utilization 17 (2017) 273–283 patterns of the samples were measured with Philip PW 1820 diffractometer to determine the crystal phase and structure of the incorporated active metals. Nitrogen adsorption–desorption measurements (BET method) were performed at liquid nitrogen temperature (196 C) with an autosorb BET apparatus, Micromeritics ASAP 2020, surface area and porosity analyzer to determine the surface area, pore size and structure, and the pore volume. 275 XPS analyses (Thermo-Fischer K-Alpha) were carried out to obtain the chemical nature, surface composition, oxidation state, relative surface compositions and the type of interaction between metal and support. The XPS was equipped with monochromatised AlKa source and the resulting samples spectra were analyzed using the Avantage software for peak ﬁtting and identiﬁcation of chemical state. The reduction behavior and active metal dispersion of the catalysts was studied using a Thermo Finnigan TPD/R/O 1100 Fig. 1. (a, d) XHR-SEM image of ZSM-5 and CZOx/Z; (b, e) STEM image of ZSM-5 and CZOx/Z; (c, f) EDX spectra of ZSM-5 and CZOx/Z. (g, h, i) CZOx/Z EDX mapping scan of Cu, Zn and O, respectively; (j) TEM image of ZSM-5; (k) TEM image of CZOx/Z; (l) HR-TEM image of CZOx/Z. 276 O.B. Ayodele et al. / Journal of CO2 Utilization 17 (2017) 273–283 equipped with a thermal conductivity detector and a mass spectrometer. Typically, 20 mg catalyst was placed in the Ushaped quartz tube. Catalyst samples were degassed under a ﬂow of nitrogen at 200 C to remove traces of water and impurities from the catalyst pores. H2 temperature program reduction (TPR) was performed using 5% H2/N2 with a ﬂow rate of 20 ml/min and heating from 40 to 990 C at 5 C min1. The acidity of the catalysts was analyzed by using temperature programmed desorption (NH3TPD). The sample was pretreated at 300 C for 2 h in He and cooled to 50 C. After being saturated with NH3, the sample was purged with He to remove the physisorbed NH3. The TPD measurements of desorbed NH3 were conducted in ﬂowing He from 60 C to 970 C at a heating rate of 10 C min1. All ﬂow rates of He mentioned above were set to 20 ml min1. The basicity test was carried using temperature programmed desorption (TPD-CO2). The sample was pretreated under the ﬂow N2 gas (30 ml/min) at 150 C for 40 min, followed by adsorption with CO2 gas for 60 min at room condition. The excess of CO2 were subsequently ﬂushed out by ﬂowing N2 gas prior to the analysis. The desorption of the CO2 from the basic sites of the catalyst were identiﬁed by TCD under helium gas (30 ml/ min) ranging from 50 C to 900 C at a heating rate of 10 C min1. Both the NH3-TPD and TPD-CO2 analysis were carried out using Thermo Finnigan (model TPDRO 1100 series). 2.4. Catalytic activity measurements The CO2 hydrogenation reaction was performed in a ﬁxed-bed microreactor (PID Eng & Tech). In a typical experiment, 0.2 g of the synthesized CZOx/Z catalyst was sandwiched between quartz wools to ensure an isothermal temperature zone around the catalyst and gently loaded into a stainless steel tube reactor. Prior to the reaction, the calcined CZOx/Z catalyst was reduced in situ using 20 ml min1 of 5% H2 in He at 250 C for 4 h under atmospheric pressure. After the reduction step, a feed consisting of a mixture of H2/CO2 (molar ratio of 3:1) was fed to the reactor and the reaction was performed at 250 C and 2.25 MPa for 10 h. All post-reactor lines and valves were heated to 180 C to prevent condensation. The feed and gaseous products were analyzed by an on-line gas chromatograph (Agilent 7890A) equipped with two TCD detectors as well as HayesepQ and molsieve columns for analyses of H2 and permanent gases. Methanol and other hydrocarbons were analyzed using a DB-1 column and a FID detector. CO2 conversion and reaction products selectivity are deﬁned as follows: CO2 conversion ¼ %Si ¼ moles ofCO2in moles of CO2out moles of CO2in ni n S i ¼ 1 products 100 ð1Þ ð2Þ where S and i are selectivity and species, respectively. 3. Results and discussion 3.1. Characterization results 3.1.1. Morphology, composition and structure The morphology of the ZSM-5 catalyst support in Fig. 1a showed that the ZSM-5 crystals/particles were highly crystalline and tightly packed which is typical of ZSM-5 zeolite types. For the purpose of clarity and elemental composition analysis, STEM image of a representative crystal was taken as shown in Fig. 1b. The spectra of elemental composition of the crystal in Fig. 1c showed that Al, Si and O are the constituents with signiﬁcantly high Si/Al Table 1 Elemental composition of ZSM-5 and CZOx/Z. Elemental composition (%) Sample ZSM-5 CZOx/Z Si 45.63 44.81 Al 4.32 2.11 O 50.05 39.49 Cu – 9.88 Zn – 3.71 Si/Al 10.56 21.24 ratio (Table 1) which is characteristics of ZSM-5. After the incorporation of the CuOx and ZnOx catalyst precursors into the ZSM-5 support, the morphology of CZOx/Z catalyst in Fig. 1d showed approximately spherical Cu and ZnO nanoparticles which are arranged in an alternating fashion and randomly distributed to form porous aggregates. This morphology is typical of industrial bulk catalyst system . The STEM image of CZOx/Z in Fig. 1e showed the Cu/ZnO arrangement in a typical ZSM-5 particle both in the inside and on the external surface of the particle. The EDX scan of the CZOx/Z STEM in Fig. 1f conﬁrmed the presence of Cu and Zn and their compositions are shown in Table 1. The sum of Cu and Zn in Table 1 is 13.59% which is marginally less than the calculated 15%. This variation might possibly due to the effect of hydration at the CZOx/Z synthesis stage, or due to the fact that EDX analysis is a point function technique [32,33]. The elemental mapping for Cu, Zn and O are shown in Fig. 1(g–i), respectively. The Cu mapping appears more conspicuous that the Zn obviously due to the difference in their ratio (70:30) at the synthesis stage. It is important to note that both Cu and Zn have high density in the same region in the map. This suggests that there is an effective interaction between the two incorporated metals as would be further elucidated in the XPS results. Furthermore, it is obvious that in those regions where both Cu and Zn showed high density in Fig. 1(g–h), the O scan in Fig. 1i showed lower O density which implied that the oxalate ion (C2O42) was effective in the reduction of metal oxide (e.g. CuO ! Cu2O ! Cu) and also able to constrain the electro-oxidation of reduced metal/metal oxide during the synthesis stage via the adsorption of C2O42[28,34]. This observation is supported by our previous study where oxalate anion was reported to have constrained the electro-oxidation of Ni  and also the works of Al-Dalama and Stanislaus  where chelating ligands from EDTA were able to constrain electrooxidation of Mo in Mo/SiO2–Al2O3 catalyst. Dong et al.  also reported that NaBH4 was effective in the reduction of CuO ! Cu2O ! Cu as the NaBH4 concentration increases. In all these studies, the TPR results showed that the effect of active metal functionalized with oxalate ligand, EDTA or NaBH4 lead to highly easily reducible ﬁne metal particles sizes at lower temperatures due to presence of limited (free) oxygen. According to a review by Liu et al.  on the recent advances in catalysts for methanol synthesis via hydrogenation of CO and CO2, catalyst with larger surface area, ﬁne particle size, and a high dispersion of active sites are essential irrespective of the synthesis method. The TEM image of ZSM-5 is shown in Fig. 1j, while Fig. 1k showed that the active metals were well dispersed on the ZSM-5 support. Furthermore, the HR-TEM in Fig. 1l showed that the well dispersed active metal were ultra-ﬁne particles in the range of 8–15 nm. Previous studies have shown that chemical reduction/functionalization is a promising and feasible alternative for preparing ultraﬁne copper-based catalysts for CO2 hydrogenation into methanol . 3.1.2. Textural properties One of the most important factors to be considered in the catalysts design for CO2 hydrogenation is enhanced textural properties which in turn guarantees ultraﬁne particle size O.B. Ayodele et al. / Journal of CO2 Utilization 17 (2017) 273–283 277 Table 2 Textural properties of ZSM-5 and CZOx/Z. Sample t-Plot Micropore Area (m2/g) t-Plot External Surface Area (m2/g) BET Surface Area (m2/g) t-Plot Micropore Volume (cm3/g) t-Plot External Volume (cm3/g) Total Pore Volume (cm3/g) BJH Pore Diameter (nm) ZSM-5 CZOx/Z 274.7 301.5 73.2 209.5 347.9 511.0 0.135 0.203 0.037 0.147 0.17 0.35 2.7 10.8 distribution and higher metal dispersion that can increase the rate of diffusions of reactant/product through the pore thus inhibiting the deactivation caused by agglomeration of the active sites . The textural properties in Table 2 showed that there is conspicuous enhancement (almost doubled) in the textural properties (BET surface area, total pore volume and pore diameter) of CZOx/Z compared to the ZSM-5 starting material. Typically what is frequently reported in the literature after impregnation/incorporation of metals/metal oxides into supports is reduction in the textural properties due to partial blocking of the pores by the active metals [10,11]. Furthermore it is obvious that there is considerable development of mesopore structure as seen in the BJH pore diameter that increased from 2.70 nm in ZSM-5 to 10.8 nm in CZOx/Z leading to eventual formation of hierarchical pore structure (Fig. 2a). Similarly, the percentage of external surface (volume) to total surface area (pore volume) increased from 21% in ZSM-5 to 41% in CZOx/Z. This textural property enhancement is ascribed to the protonic effect of oxalic acid used to functionalize Cu and Zn at the synthesis stage. Typically, aluminosilicates such as clay minerals and zeolites undergo varying extents of dealumination under acidic or thermal treatment leading to the removal of extra framework and framework alumina, respectively which results into enhanced textural properties with high Si/Al ratio (Table 1) . The enhancement in the CZOx/Z textural properties is further corroborated by the N2 isotherms in Fig. 2b. The isotherms of both ZSM-5 and CZOx/Z reﬂected steady increase in adsorption strengths with increase in the relative adsorption pressure (P/Po) up to 0.9 for ZSM-5 and 0.76 for CZOx/Z indicating the existence of the micropores typical of Type I isotherms for microporous materials. While ZSM-5 showed a nearly negligible Fig. 3. XRD patterns of ZSM-5 and CZOx/Z. uptake at P/Po = 0.9–1.0, CZOx/Z exhibited a very conspicuous N2 steep uptake at P/Po = 0.76–1.0 which was attributed to the interparticle voids formed by agglomeration of the nano-sized CZOx/Z crystals. In addition, the CZOx/Z hysteresis loop at P/Po = 0.76–1.0 steadily conforms to Type IV isotherm which conﬁrmed an increase in the mesopore formation. Similarly the increase in the amount of N2 adsorbed/desorbed indicated there is increase in the pore volume as seen in Table 2. 3.1.3. XRD The X-ray diffraction patterns of ZSM-5 support is shown in Fig. 3 with its characteristics distinctive peaks at 2u values of 7.8 , 8.9 , 22.2 , 23.8 , 24.9 , 26.8 , 30.1 and 45.5 . There is Fig. 2. (a) Pore size distribution of ZSM-5 and CZOx/Z, (b) N2 isotherm of ZSM-5 and CZOx/Z. 278 O.B. Ayodele et al. / Journal of CO2 Utilization 17 (2017) 273–283 marginal variation (i.e. crystallinity loss) in the diffraction pattern of CZOx/Z catalyst compared to ZSM-5 after the incorporation of CuOx and ZnOx catalyst precursors which implied that the synthesis protocol does not destroy the ZSM-5 crystallographic structure, thus the zeolite structures remained largely intact . The marginal loss of crystallinity was ascribed to the weak protonation effect of oxalic acid during the synthesis stage. Therefore, the enhanced textural properties seen the BET results of CZOx/Z could be largely due to removal of partly occluded organic and non-zeolitic matters. There are no distinctive diffractions peaks for copper or zinc oxides (except for a weak amorphous peak at 36.5 which could be ascribed to (111) plane of octahedral Cu2O which is typical of high degree of active metal dispersion or low active metal concentration. Zhang et al.  also reported similar observation in a study where Cu-ZSM-5 with low Cu concentration (2.8%) was prepared by ion-exchange. In order to ascertain the reason for the nonappearance of metal/metal oxides peaks in this study, some samples of uncalcined CZOx/Z catalyst was calcined at 450 C and characterized with XRD. The result is shown in Fig. S1 with characteristic peaks of CuO at 2u values of 35.6 , 38.8 and 66.3 corresponding to (-111/002), (111) and (311) plane, respectively [39,40]. Similarly, poorly grown ZnO peaks at 2u values of 48.6 and 68.2 which corresponds to (102) and (201) ZnO hexagonal phase according to JCPDF No. 36-1451  were also observed. The appearance of these peaks after calcination at relatively higher temperature is undoubtedly due to metal oxide crystal growth resulting from agglomeration of CuO and ZnO particles. This conﬁrmed that the absence of metal oxide peaks in CZOx/Z is obviously due to high active metal dispersion which guaranteed that the synthesis protocol is expedient. After the incorporation of the CuOx and ZnOx catalyst precursors into the ZSM-5 structure, RS band c.a. 298 cm1 and 387 cm1 were observed to shift to lower wavenumber of 290 cm1 and 373 cm1, respectively. While the peak intensity becomes stronger in the former, the latter loss some level of crystallinity and the peak tip becomes broader. The increase in intensity of the peak at 290 cm1 can be ascribed to overlapping of Cu2O, while the shifts of 298 cm1 and 387 cm1 to lower wavenumbers were ascribed to the marginal reduction in average particle size of CZOx/Z due to the inﬂuence of oxalate ligand functionalization as seen in the XHRSEM and BET results. This effect of crystallite size on the Raman spectra has been reported by Akgul et al.  and Xu et al.  that as the Cu-oxide nanoparticles grain size decreases, the Raman peaks shift to lower wavenumber and become broader owing to size effects. Thus, Raman peaks shift to higher wavenumbers as grain size increases and vice versa. A new Raman band at 468 cm1 due to the bending mode of symmetric Cu-oxo stretch (ns) of a mono-m-oxo bridged dicopper core was observed . In addition, there is a distinctive high intensity broad hump centered around 579 cm1 which clearly indicated the presence of Cu2O phase [40,43]. This showed that 3.1.4. Raman spectroscopy Since the XRD patterns did not show any distinctive peak for the incorporated metal/metal oxide, Raman spectroscopy (RS) which is a powerful method for the identiﬁcation of different metal oxides through the change in polarizability was performed to ascertain the phase of copper oxide since RS is very sensitive to both copper oxide phases of Cu2O and CuO . The Raman spectrum of CZOx/Z with excitation line at 325 nm is compared with the spectrum of pure ZSM-5 as shown in Fig. 4. Accordingly, the RS band c.a. 298 cm1 and 387 cm1 are assigned to bending mode of 6membered ring and 5-membered building unit of ZSM zeolites structure, respectively. Similarly, the RS bands at 440 cm1, 470 cm1 and the 802 cm1 are associated with vibration of 4membered ring related to the framework symmetric stretching vibration in ZSM-5 . Fig. 4. Raman Spectra of ZSM-5 and CZOx/Z. Fig. 5. (a) High-resolution XPS scan of Cu 2p spectra of CZOx/Z. (b) High-resolution XPS scan of Zn 2p spectra of CZOx/Z. High-resolution XPS scan of O 1 s spectra of (c) ZSM-5 and (d) CZOx/Z. O.B. Ayodele et al. / Journal of CO2 Utilization 17 (2017) 273–283 279 functionalization of the active metals with oxalate anion (C2O42) was effective in reducing CuO as well as constraining electrooxidation of reduced species, more so that the characteristics Raman Bg mode of CuO peak at 604 cm1 is not seen. The most intense B-type carbonate band centered at 1100 cm1 can be assigned to overlapping bands of n1CO32 from oxalate ligand and peaks of Zn2+ from ZnO particles which normally gives peak at 1098 cm1 [44,45]. The reduction and electro-oxidation constraints imposed by the oxalate anion functionalization that promotes the formation of Cu+ which is synonymous to the promoter effect of Zr in a Cu/Zn catalyst that results into synthesis of a new copper oxide phase and promotes the formation of Cu+ ions for methanol synthesis at low temperatures and pressures . 3.1.5. XPS The high resolution scan for the Cu 2p core level spectrum for CZOx/Z is shown in Fig. 5a with two characteristics peaks at 932.8 eV and 951 eV which corresponds to the Cu 2p3/2 and Cu 2p1/ 0 + 2, respectively, and are typical of Cu and Cu . This was further supported by the observed Cu 2p core level split spin-orbit components (D Cu 2p) of 18.2 eV. However, the presence of a very weak satellite at 944.3 eV suggested that there is substantial amount of Cu+ oxidation state. It is important to note that the Cu2+ satellite peaks were totally absent in Fig. 5a which conﬁrmed that the oxalate functionalization in the CZOx/Z synthesis protocol was indeed effective in the reduction of CuO ! Cu2O ! Cu as well as guaranteeing the electro-oxidation constraints during calcination. This observation supports both the STEM-EDX mapping and the Raman spectrum that show low O density (Fig. 1i) and the presence of Cu2O, respectively. For clarity and comparison purpose, another CZOx/Z was synthesized following the same protocol but without oxalate functionalization (CZOx/Z**), their spectra were plotted and compared in Fig. S2 (Supporting information). There are two important distinguishing features, ﬁrstly, there is a shift in the binding energy peaks of Cu 2p of CZOx/Z** to higher BE of 933.5 eV and 953.2 eV corresponding to the Cu 2p3/2 and Cu 2p1/2, respectively. Secondly, there are very conspicuous observable co-joined collection of satellite features at 941 eV and 943 eV for Cu 2p3/2 peak as well as at 961.7 eV for Cu 2p1/2 peak. Both of these observation matches well with the data reported for the Cu2+ from CuO [39,40], and they further conﬁrmed that the oxalate functionalization in the CZOx/Z synthesis protocol ensured both reduction of CuO and the electro-oxidation constraint during synthesis thus leading to ultraﬁne particles (as seen in the HRTEM) with reasonably weak metal support interaction. The high-resolution XPS spectra of the Zn 2p orbital peak is shown in Fig. 5b with two characteristics distinct peaks at binding energies of 1021.1 and 1044.2 eV corresponding to the Zn 2p3/2 and Zn 2p1/2, respectively and it is consistent within the range reported in the literature for Zn2+ from ZnO [47,48]. However, the characteristics peak at 2p3/2 and 2p1/2 appears shifted to lower binding energies compared to the values reported in those literature for ZnO which implied comparable weaker metalsupport-interaction due to instances of ZnO reduction, especially considering the Zn 2p peak split spin-orbit components (D Zn 2p) of 23.1 eV which is typical of Zn0. (Fig. S3 (Supporting information) shows comparison between CZOx/Z and CZOx/Z** (without oxalate functionalization)). This further corroborated that the oxalate anion functionalization is effective at reducing the metal oxide and constrained electro-oxidation of reduced species. This was further supported by the O 1 s spectra of ZSM-5 and CZOx/Z (Fig. 5c,d) which showed decrease in the ratio of lattice O/ adsorbed from 0.72 in ZSM-5 to 0.5 in CZOx/Z. Furthermore, the FWHM lattice O showed substantial reduction (0.68 eV) from 3.13 eV in ZSM-5 to 2.45 eV in CZOx/Z due to inﬂuence in bonding Fig. 6. H2 temperature programmed reduction proﬁle of CZOx/Z catalyst. arrangement from the incorporated CuOx and ZnOx at the synthesis stage and adsorbed C2O42 which restrained the electro-oxidation of reduced species [34,49]. Similarly, the FWHM of the adsorbed O showed a signiﬁcant increment of 1.18 eV in CZOx/Z which could be attributed to the surface adsorbates which are a signiﬁcant feature due to the surface sensitivity of XPS as well as hydrated C2O42 from oxalate functionalization. Thus, it is a combination of materials adsorbed on the surface and starting materials (CuOx and ZnOx) that resulted in the larger FWHM . 3.1.6. Temperature programmed reduction The TPR proﬁle of CZOx/Z is shown in Fig. 6. The characteristic copper oxide reduction peaks which usually gave broad peak spanning from 200 to 400 C with a maxima around 300 C  was seen to have shifted to a very much lower reduction temperature with three peaks. The ﬁrst minuscule peak at 200 C was ascribed to readily reducible surface species, while the peaks at 207 and 265 C were ascribed to Cu2+ ! Cu+ and Cu+ ! Cu , respectively. The broad reduction peak ranging from 400 to about 700 C with a maxima at 550 C is attributed to reduction of ZnO which otherwise shows reduction peak above 800 C  and it is rarely reported in CO2 hydrogenation studies. The shift to these peaks to comparably lower reduction temperature was due to the oxalate ligand functionalization which was seen in the XPS result to have partially reduced copper oxides and further constrained the electro-oxidation of the partially reduced species. This observation Fig. 7. (a) NH3, (b) CO2 temperature programmed desorption of CZOx/Z catalyst. 280 O.B. Ayodele et al. / Journal of CO2 Utilization 17 (2017) 273–283 is similar to the report of Dong et al.  which showed a shift in reduction temperature to 427 and 454 K (219 and 234 C) when the CuZnO/ZrO2 catalyst was prepared via precipitation-reduction method using NaBH4 compared to 469 K (243 C) recorded using conventional co-precipitation method without NaBH4. These results suggested that chemical reduction of metal oxides are effective and prospective, however, based on the results shown here, it appears oxalate ligand functionalization is more prospective more so that ZrO2 support used in that study favors high metal reducibility compared to ZSM-5, and it is more expensive. 3.1.7. Acidity and basicity studies The acidity and basicity proﬁle of CZOx/Z catalyst is shown in the NH3 and CO2 temperature programmed desorption (TPD) plots in Fig. 7a–b with three distinctive peaks, respectively. Form the NH3-TPD plot, the peak a at 365 C corresponds to the aluminum centers of ZSM-5, while the peak ß at 447 C is due to higher degree of metal (Cu and Zn) oxide ﬁne particle size dispersion (Fig. 1j–k) leading to higher desorption of the physisorbed NH3 from the acid sites on the catalyst surface. The last peak g at 682 C was ascribed to strong acid site within the pores of CZOx/Z catalyst. The peak g is relatively less intense but broader compared to the ﬁrst two peaks, which implied that there is lower desorption of the physisorbed NH3 from the acid sites of the nano metal (Cu and Zn) oxide/oxalate particles within the pore of the CZOx/Z catalyst. The amount of desorbed physisorbed NH3 from the acid sites in Table 3 shows that the peak ß has the highest contribution, and according to previous discussions, it was due to the oxalate ligand functionalization. The catalyst showed a very substantial value of 8.96 mmol/m2 for the density of acid sites which according to a previous report  is signiﬁcantly promising for the formation of methyl formate via acid-catalyzed esteriﬁcation of formic acid and methanol. The three peaks at 329, 387 and 682 C in the CO2–TPD for the basicity studies of the CZOx/Z catalyst in Fig. 7b can be ascribed to weak (d), moderate (e) and strongly basic (l) sites . The three peaks appear at a comparably higher desorption temperature compared to what was reported in the recent literature, for example Zhang et al.  reported 88, 118 and 155 C for Cu/ZnO/ Al2O3/ZrO2 catalyst, while Witoon et al.  reported 65, 145 and 230 C for Cu supported on monoclinic zirconia which showed more basic sites compared to amorphous or tetragonal zirconia. Other studies also show 126, 175 and 256 C for Cu/Zn/Al-Mn catalysts  and 120, 166 and 237 C for a ﬂuorine modiﬁed Cu/ Zn/Al/Zr hydrotalcite-like catalyst  for the peaks d, e, l, respectively. This shift to higher desorption temperature in this study signiﬁed that the basic sites were strongly bonded. In those studies, the peaks d, e, l were ascribed to surface hydroxyl groups, M–oxygen pairs (M = Cu, Zn and Al), and coordinatively unsaturated O2 ions (low coordination oxygen atoms), respectively. The peaks d, e, l were sharp and distinct thus there is no need for Fig. 8. CO2 conversion and product distribution ﬂow at 250 C and 2.25 MPa for 10 h. deconvolution into three Gaussian peaks as practiced in those studies. The number of total basic sites from Table 3 is 1117.31 mmol/g which is far higher than 1009.06 mmol/g , 289.9 mmol/g  and 257.4 mmol/g  previously reported. The sharpness, distinctiveness and increased in basicity in this study was ascribed to the oxalate ligand functionalization that forms Moxalate pairs and coordinatively unsaturated C2O42 anions. This observation is at par with the result of Wu et al.  on ﬂuorinemodiﬁed Mg–Al mixed oxides which showed that the formation of metal–ﬂuorine pairs and the unsaturated F ions increased the amounts of the moderately and strongly basic sites. Therefore CZOx/Z catalyst is expected to exhibit outstanding CO2 conversion and much higher CH3OH selectivity compared to those cited literature since enhanced basicity has been reported to favor methanol synthesis [10,11,51,52]. 3.1.8. Catalytic activity and selectivity The proﬁle of CO2 conversion and the products molar ﬂow in Fig. 8 shows that the CO2 conversion at 60 min time-on-stream (TOS) is 15.55% and slightly increased to 19.13% at 240 min. Beyond 240 min, the CO2 conversion steadied around 20.4% until 600 min. From literature, it is generally accepted that the coordination, chemisorption, and activation of CO/CO2 and the homogeneous splitting of hydrogen take place on Cu0 or Cu+ [7,13]. Based on this, it appears that as the reaction proceeds in this study, part of the formed methanol further reduced remnant Cu-oxides especially those in the interstices of the ZSM-5 support that were not properly reduced during hydrogen reduction step. Thus, the progressive reduction of these Cu-oxides enhanced the CO2 conversion from 15.55 to 20.4%. It is important to recall that Table 3 Acid and basic properties of CZOx/Z catalyst. NH3 – TPD of CZOx/Z catalyst Peak ID T [ C] Integral [mVs] a 365 447 682 17619.7 108792.8 19255.6 ß g Number of total acid sites = 4581.89 mmol/g. Number of total basic sites = 1117.31 mmol/g. Density of acid sites = 8.96 mmol/m2. Density of basic sites = 2.19 mmol/m2. CO2 – TPD of CZOx/Z catalyst Total acid sites [mmol/g] 554.37 3421.67 605.85 [%] Peak ID T [ C] Integral [mVs] 12.11 74.69 13.22 d e l 329 387 682 22889.52 31698.96 26528.79 Total basic sites [mmol/g] 315.28 436.62 365.41 [%] 28.22 39.08 32.7 O.B. Ayodele et al. / Journal of CO2 Utilization 17 (2017) 273–283 CZOx/Z catalyst was reduced prior to experimental at 250 C to prevent the agglomeration of surface active sites since Fujita et al.  has established that lower reduction temperature is beneﬁcial for improving copper dispersion and activity for the methanol synthesis. The authors further showed that activity of a coprecipitated Cu/ZnO catalyst depended on the procedure for the reduction and the reductant, and that reduction with methanol at 443 K (228.33 C) (which is in the neighborhood of the reaction temperature in this study) showed higher CO2 conversion and methanol selectivity than reduction with hydrogen. The CO2 conversion in this study is comparably higher than most of the values reported in literature, for example, Bahruji et al.  reported a range of 0.7–10.7% for different Pd/ZnO catalysts systems. Other authors [10–12,51,52] also showed CO2 conversions in the range of <1–20% using Cu/ZnO catalysts on different supports. In all these studies, strong basic site were acknowledged as being favorable for the CO2 conversion. Therefore, in addition to the progressive methanol reduction of active metals in this study, the high CO2 conversion can be ascribed to the strong basic sites (Table 3) and high active metal reducibility shown in (Fig. 6) which is consistent with previous studies [7–11,29]. From Fig. 8, the molar ﬂow of methanol was initially 167.36 mol/ h at 60 min TOS and increased to 187.47 mol/h at 120 min TOS as the CO2 conversion increased. Beyond 300 min, the methanol ﬂow decreased even though the CO2 conversion appeared somewhat steady. This reduction was ascribed to the formation of MF as its molar ﬂow which was zero at the ﬁrst 60 min TOS began to increase until 118.65 mol/h at 600 min TOS. This is supported by a previous study  which showed that during methanol synthesis there was endothermic dehydrogenation of methanol to methyl formate (MF). Other mechanism for the production of MF besides dehydrogenation of methanol is via acid-catalyzed esteriﬁcation of formic acid and methanol, or base-catalyzed reaction of methanol and carbon monoxide [13,50]. Consequently, since CZOx/Z catalyst has been shown to possess both active acid and basic sites (Fig. 7, Table 2), and the methanol ﬂow was also observed to reduce slightly, it is possible that these three MF production routes played certain roles in this study. However, the contribution(s) based on the presence of acid and basic sites seems overriding over any contribution from dehydrogenation of methanol to MF. This is because according to Eq. (3), a mole of MF requires two moles of methanol stoichiometrically but the amount of methanol reduction between 120 and 600 min was only 11.93 mol/h which is far lower compared to the 108 mol/h increase in MF production. Similarly, since the number of acid site is more 281 than 4 times higher than the number of basic sites, we concluded that acid-catalyzed esteriﬁcation of methanol and formic acid as well as dehydrogenation of methanol are the likely main mechanisms of MF production. 2CH3 OH ! C 2 H4 O2 þ 2H2 ð3Þ The proﬁle of product selectivity in Fig. 9 showed that the selectivity of methanol is about 97.16% at 60 TOS when there was no MF formation, but it decreased to 93.24% at 120 min TOS when MF was ﬁrst noticed. This high methanol selectivity is comparably higher than what have been reported in literature, for example, Zhang et al.,  reported a range of 55.2–61.5% selectivity over Cu/ Zn/Al/Zr with varying Al content and the selectivity increases with reduction in the Al content. Thus, the high selectivity of methanol in this study might have contributions from the dealumination of CZOx/Z catalyst during the synthesis stage leading to higher Si/Al ratio in Table 1. This phenomenon was ascribed to the expedient functionalization of the active metals with oxalate ligand at the synthesis stage which guarantee high dispersions and reducibility of active metals, enhanced textural properties and high number of acid and basic sites as seen in the HR-TEM, BET, Raman spectroscopy, TPR and CO2/NH3-TPD results. As the reaction continues, methanol selectivity steeply reduced to 64.64% at 180 min, while the MF selectivity swiftly increased to 34.12% at 180 min and steadied at about 39.8% at 540 min and beyond. This observation suggested that the secondary reduction of remnant active metal oxide with methanol as the reaction progresses which proceeds with dehydrogenation of methanol into MF also increases the number of acid sites and possibly decrease the number of basic sites. There is also an instance of methanation of CO2 in somewhat Fischer-Tropsch process, but the inﬂuence is very marginal. Similarly, the reverse water gas shift reaction (CO2 + H2 ! CO + H2O; DH = +9 kcal/mole) which typically competes with methanol selectivity in virtually all the reported studies were not observed in this study, and we ascribed this to the high density of acid sites since basic sites has been found to favor CO production especially via parallel formate dissociation mechanism . 4. Conclusion Expediently synthesized ZSM-5 supported oxalate ligand functionalized Cu/ZnO catalyst (CZOx/Z) achieved excellent CO2 hydrogenation into methanol with CO2 conversion ranging from 15.5 to 20.4% at 180 and 600 min time-on-stream (TOS), respectively. The enhanced CO2 conversion was ascribed to excellent ultraﬁne active metal particle sizes with enhanced porosity, high reducibility and strong basic site. The increase in the CO2 conversion with prolonged TOS was ascribed to the progressive reduction of unreduced active metals at the reduction stage with methanol which also proceeds with the formation of methyl formate (MF) at the CZOx/Z catalyst acid sites via dehydrogenation of methanol and acid esteriﬁcation of formic acid with methanol. The formation of MF reduces the selectivity of methanol from 97.16% to 64. 64% at 180 min TOS. There was also insigniﬁcant instance of methanation process over the entire TOS. The products selectivity at 600 min TOS were 58.9, 39.8 and 1.2% for methanol, MF and methane, respectively. Acknowledgement Fig. 9. Product selectivity at 250 C and 2.25 MPa for 10 h (methanol and methyl formate are read on the primary Y-axis and methane is read on the secondary Yaxis). The authors sincerely acknowledge the ﬁnancial support from the Mitsubishi Corporation Education Trust Fund, University Teknologi PETRONAS, Malaysia. The Ministry of Higher Education Malaysia research grant FRGS/2/2014/SG01/UTP/02/2 is also appreciated. 282 O.B. Ayodele et al. / Journal of CO2 Utilization 17 (2017) 273–283 Appendix A. Supplementary data Supplementary data associated with this article can be found, in the online version, at http://dx.doi.org/10.1016/j.jcou.2016.11.016.   References   O.B. Ayodele, H.F. Abbas, W.M.A.W. Daud, Hydrodeoxygenation of stearic acid into normal and iso-Octadecane biofuel with zeolite supported palladiumOxalate catalyst, Energy Fuels 28 (9) (2014) 5872–5881.  O.B. Ayodele, H.F. Abbas, W.M.A.W. Daud, Preparation and characterization of zeolite supported ﬂuoropalladium oxalate catalyst for hydrodeoxygenation of oleic acid into parafﬁnic fuel, Ind. Eng. Chem. Res. 53 (2) (2014) 650–657.  O.B. Ayodele, H.F. Abbas, W.M.A.W. Daud, Catalytic upgrading of oleic acid into biofuel using Mo modiﬁed zeolite supported Ni oxalate catalyst functionalized with ﬂuoride ion, Energy Convers. Manage. 88 (2014) 1111–1119.  O.B. Ayodele, H.U. Farouk, J. Mohammed, Y. Uemura, W.M.A.W. Daud, Effect of precursor acidity on zeolite supported Pd catalyst properties and hydrodeoxygenation activity for the production of biofuel, J. Mol. Catal. A Chem. 400 (2015) 179–186.  O.B. Ayodele, O.S. Togunwa, H.F. Abbas, W.M.A.W. Daud, Preparation and characterization of alumina supported nickel-oxalate catalyst for the hydrodeoxygenation of oleic acid into normal and iso-octadecane biofuel, Energy Convers. Manage. 88 (2014) 1104–1110.  M. Behrens, F. Studt, I. Kasatkin, S. Kuhl, M. Havecker, F. Abild-Pedersen, S. Zander, F. Girgsdies, P. Kurr, B.L. Kniep, M. Tovar, R.W. Fischer, J.K. Norskov, R. Schlogl, The active site of methanol synthesis over Cu/ZnO/Al2O3 industrial catalysts, Science 336 (6083) (2012) 893–897.  X.-M. Liu, G.Q. Lu, Z.-F. Yan, J. Beltramini, Recent advances in catalysts for methanol synthesis via hydrogenation of CO and CO2, Ind. Eng. Chem. Res. 42 (2003) 6518–6530.  X. Chen, X. Yang, Bioinspired design and computational prediction of iron complexes with pendant amines for the production of methanol from CO2 and H2, J. Phys. Chem Lett. 7 (6) (2015) 1035–1041.  R.J. da Silva, A.F. Pimentel, R.S. Monteiro, C.J.A. Mota, Synthesis of methanol and dimethyl ether from the CO2 hydrogenation over CuZnO supported on Al2O3 and Nb2O5, J. CO2 Util. 15 (2016) 83–88.  X. Dong, F. Li, N. Zhao, F. Xiao, J. Wang, Y. Tan, CO2 hydrogenation to methanol over Cu/ZnO/ZrO2 catalysts prepared by precipitation-reduction method, Appl. Catal. B: Environ. 191 (2016) 8–17.  T. Witoon, J. Chalorngtham, P. Dumrongbunditkul, M. Chareonpanich, J. Limtrakul, CO2 hydrogenation to methanol over Cu/ZrO2 catalysts: effects of zirconia phases, Chem. Eng. J. 293 (2016) 327–336.  H. Bahruji, M. Bowker, G. Hutchings, N. Dimitratos, P. Wells, E. Gibson, W. Jones, C. Brookes, D. Morgan, G. Lalev, Pd/ZnO catalysts for direct CO2 hydrogenation to methanol, J. Catal. 343 (2016) 133–146.  Y. Chen, S. Choi, L.T. Thompson, Ethyl formate hydrogenolysis over Mo2C-based catalysts: towards low temperature CO and CO2 hydrogenation to methanol, Catal. Today 259 (Part 2) (2016) 285–291.  J. Ye, C. Liu, D. Mei, Q. Ge, Active oxygen vacancy site for methanol synthesis from CO2 hydrogenation on In2O3(110): a DFT study, ACS Catal. 3 (6) (2013) 1296–1306.  S. Natesakhawat, J.W. Lekse, J.P. Baltrus, P.R. Ohodnicki, B.H. Howard, X. Deng, C. Matranga, Active sites and structure–activity relationships of copper-based catalysts for carbon dioxide hydrogenation to methanol, ACS Catal. 2 (8) (2012) 1667–1676.  L.C. Grabow, M. Mavrikakis, Mechanism of methanol synthesis on Cu through CO2 and CO hydrogenation, ACS Catal. 1 (4) (2011) 365–384.  Y. Hartadi, D. Widmann, R.J. Behm, Methanol formation by CO2 hydrogenation on Au/ZnO catalysts Effect of total pressure and inﬂuence of CO on the reaction characteristics, J. Catal. 333 (2016) 238–250.  A.A. Kiss, J.J. Pragt, H.J. Vos, G. Bargeman, M.T. de Groot, Novel efﬁcient process for methanol synthesis by CO2 hydrogenation, Chem. Eng. J. 284 (2016) 260–269.  H. Yang, P. Gao, C. Zhang, L. Zhong, X. Li, S. Wang, H. Wang, W. Wei, Y. Sun, Core– shell structured [email protected] and Cu/[email protected] catalysts for methanol synthesis from CO2 hydrogenation, Catal. Commun. 84 (5) (2016) 56–60.  Y. Yang, M.G. White, P. Liu, Theoretical study of methanol synthesis from CO2 hydrogenation on metal-Doped Cu(111) surfaces, J. Phys. Chem. C 16 (1) (2012) 248–256.  Y. Zhang, L. Zhong, H. Wang, P. Gao, X. Li, S. Xiao, G. Ding, W. Wei, Y. Sun, Catalytic performance of spray-dried Cu/ZnO/Al2O3/ZrO2 catalysts for slurry methanol synthesis from CO2 hydrogenation, J. CO2 Util. 15 (2016) 72–82.  N.A.M. Zabidi, S. Tasfy, M.S. Shaharun, Effects of Nb promoter on the properties of Cu/ZnO/SBA-15 catalyst and performance in methanol production, Key Eng. Mater. 708 (2016) 94–97.  S. Belin, C.L. Bracey, V. Briois, P.R. Ellis, G.J. Hutchings, T.I. Hyde, G. Sankar, CuAu/SiO2 catalysts for the selective oxidation of propene to acrolein: the impact of catalyst preparation variables on material structure and catalytic performance, Catal. Sci. Technol. 3 (11) (2013) 2944–2957.  B.J. Liaw, Y.Z. Chen, Liquid-phase synthesis of methanol from CO2/H2 over ultraﬁne CuB catalysts, Appl. Catal. A Gen. 206 (2) (2001) 245–256.  S.-i. Fujita, S. Moribe, Y. Kanamori, M. Kakudate, N. Takezawa, Preparation of a coprecipitated Cu/ZnO catalyst for the methanol synthesis from CO2 – effects                        of the calcination and reduction conditions on the catalytic performance, Appl. Catal. A Gen. 207 (1–2) (2001) 121–128. C.-S. Chen, W.-H. Cheng, S.-S. Lin, Study of reverse water gas shift reaction by TPD, TPR and CO2 hydrogenation over potassium-promoted Cu/SiO2 catalyst, Appl. Catal. A Gen. 238 (1) (2003) 55–67. T. Tan, M. Pavone, D.B. Krisiloff, E.A. Carter, Ab initio reaction kinetics of hydrogen abstraction from methyl formate by hydrogen, methyl, oxygen, hydroxyl, and hydroperoxy radicals, J. Phys. Chem. A 116 (33) (2012) 8431– 8443. O.B. Ayodele, K.C. Lethesh, Z. Gholami, Y. Uemura, Effect of ethanedioic acid functionalization on Ni/Al2O3 catalytic hydrodeoxygenation and isomerization of octadec-9-enoic acid into biofuel: kinetics and Arrhenius parameters, J. Energy Chem. 25 (1) (2016) 158–168. D. Jingfa, S. Qi, Z. Yulong, C. Songying, W. Dong, A novel process for preparation of a Cu/ZnO/Al2O3 ultraﬁne catalyst for methanol synthesis from CO2 + H2: comparison of various preparation methods, Appl. Catal. A: Gen. 139 (1) (1996) 75–85. W. Ning, H. Shen, H. Liu, Study of the effect of preparation method on CuOZnO-Al2O3 catalyst, Appl. Catal. A: Gen. 211 (2) (2001) 153–157. O.B. Ayodele, O.S. Togunwa, Catalytic activity of copper modiﬁed bentonite supported ferrioxalate on the aqueous degradation and kinetics of mineralization of Direct Blue 71, Acid Green 25 and Reactive Blue 4 in photoFenton process, Appl. Catal. A Gen. 470 (2014) 285–293. O.B. Ayodele, B.H. Hameed, Synthesis of copper pillared bentonite ferrioxalate catalyst for degradation of 4-nitrophenol in visible light assisted Fenton process, J. Ind. Eng. Chem. 9 (3) (2013) 966–974. O.B. Ayodele, J.K. Lim, B.H. Hameed, Pillared montmorillonite supported ferric oxalate as heterogeneous photo-Fenton catalyst for degradation of amoxicillin, Appl. Catal. A Gen. 413–414 (2012) 301–309. O.B. Ayodele, Structure and reactivity of ZSM-5 supported oxalate ligand functionalized nano-Fe catalyst for low temperature direct methane conversion to methanol, Energy Convers. Manage. 126 (2016) 537–547. K. Al-Dalama, A. Stanislaus, Temperature programmed reduction of SiO2– Al2O3 supported Ni, Mo and NiMo catalysts prepared with EDTA, Thermochim. Acta 520 (1–2) (2011) 67–74. O.B. Ayodele, Effect of phosphoric acid treatment on kaolinite supported ferrioxalate catalyst for the degradation of amoxicillin in batch photo-Fenton process, Appl. Clay Sci. 72 (2013) 74–83. L. Jin, T. Xie, S. Liu, Y. Li, H. Hu, Controllable synthesis of chainlike hierarchical ZSM-5 templated by sucrose and its catalytic performance, Catal. Commun. 75 (2016) 32–36. T. Zhang, J. Shi, J. Liu, D. Wang, Z. Zhao, K. Cheng, J. Li, Enhanced hydrothermal stability of Cu-ZSM-5 catalyst via surface modiﬁcation in the selective catalytic reduction of NO with NH3, Appl. Surf. Sci. 375 (2016) 186–195. A.S. Ethiraj, D.J. Kang, Synthesis and characterization of CuO nanowires by a simple wet chemical method, Nanoscale Res. Lett. 7 (1) (2012) 70. F.A. Akgul, G. Akgul, N. Yildirim, H.E. Unalan, R. Turan, Inﬂuence of thermal annealing on microstructural, morphological, optical properties and surface electronic structure of copper oxide thin ﬁlms, Mater. Chem. Phys. 147 (3) (2014) 987–995. Y.T. Prabhu, K.V. Rao, V.S.S. Kumar, B.S. Kumari, Synthesis of ZnO nanoparticles by a novel surfactant assisted amine combustion method, Adv. Nanoparticles 2 (1) (2013) 6. J.F. Xu, W. Ji, Z.X. Shen, W.S. Li, S.H. Tang, X.R. Ye, D.Z. Jia, X.Q. Xin, Raman spectra of CuO nanocrystals, J. Raman Spectrosc. 30 (5) (1999) 413–415. B. Balamurugan, B.R. Mehta, D.K. Avasthi, F. Singh, A.K. Arora, M. Rajalakshmi, G. Raghavan, A.K. Tyagi, S.M. Shivaprasad, Modifying the nanocrystalline characteristics—structure, size, and surface states of copper oxide thin ﬁlms by high-energy heavy-ion irradiation, J. Appl. Phys. 92 (6) (2002) 3304–3310. G.S. Mandair, M.D. Morris, Contributions of Raman spectroscopy to the understanding of bone strength, Bonekey. Rep. 4 (2015). D.A. Guzma’n-Embu’s, M. Orrego Cardozo, C. Vargas-Herna’ndez, Genomic DNA characterization of pork spleen by Raman spectroscopy, J. Appl. Phys. 114 (19) (2013) 194704. Y. Mikhlin, A. Karacharov, Y. Tomashevich, A. Shchukarev, Interaction of sphalerite with potassium n-butyl xanthate and copper sulfate solutions studied by XPS of fast-frozen samples and zeta-potential measurement, Vacuum 125 (2016) 98–105. H.-J. Choi, S.-J. Choi, S. Choo, I.-D. Kim, H. Lee, Hierarchical ZnO nanowiresloaded Sb-doped SnO2-ZnO Micrograting Pattern via Direct Imprintingassisted Hydrothermal Growth and Its Selective Detection of Acetone Molecules, Sci. Rep. 6 (2016) 18731–18932. L. Xu, B. Wei, W. Liu, H. Zhang, C. Su, J. Che, Flower-like ZnO-Ag2O composites: precipitation synthesis and photocatalytic activity, Nanoscale Res. Lett. 8 (1) (2013) 1–7. C.A. Dearden, M. Walker, N. Beaumont, I. Hancox, N.K. Unsworth, P. Sullivan, C. F. McConville, T.S. Jones, High voltage hybrid organic photovoltaics using a zinc oxide acceptor and a subphthalocyanine donor, Phys. Chem. Chem. Phys. 6 (35) (2014) 18926–18932. B. Indu, W.R. Ernst, L.T. Gelbaum, Methanol-formic acid esteriﬁcation equilibrium in sulfuric acid solutions: inﬂuence of sodium salts, Ind. Eng. Chem. Res. 32 (5) (1993) 981–985. P. Gao, F. Li, N. Zhao, F. Xiao, W. Wei, L. Zhong, Y. Sun, Inﬂuence of modiﬁer (Mn, La Ce, Zr and Y) on the performance of Cu/Zn/Al catalysts via hydrotalcite-like precursors for CO2 hydrogenation to methanol, Appl. Catal. A Gen. 468 (2013) 442–452. O.B. Ayodele et al. / Journal of CO2 Utilization 17 (2017) 273–283  P. Gao, F. Li, H. Zhan, N. Zhao, F. Xiao, W. Wei, L. Zhong, Y. Sun, Fluorinemodiﬁed Cu/Zn/Al/Zr catalysts via hydrotalcite-like precursors for CO2 hydrogenation to methanol, Catal. Commun. 50 (2014) 78–82. 283  G. Wu, X. Wang, W. Wei, Y. Sun, Fluorine-modiﬁed Mg–Al mixed oxides: a solid base with variable basic sites and tunable basicity, Appl. Catal. A Gen. 377 (1–2) (2010) 107–113.
© Copyright 2022 Paperzz